Strength Characteristics and Durability
Characteristics of Silicafume and Metakaolin
M.TechStudent,Department of Civil Engineering, Prist University, Kumbakonam Campus, Tamilnadu, India
Asst. Professor, Department of Civil Engineering, Prist University, Kumbakonam Campus, Tamilnadu, India
Abstract - Silica fume (SF) and Metakaolin are cementitious materials used as admixtures to produce high strength concrete and to reduce the permeability. Also, Silica fume is used to make durable concrete structures in combination with ordinary Portland cement. In places where insufficient or poor curing concrete structures like sea shores, underground structures which undergo severe loss of compressive strength and permeability interconnected durability, use of Metakaolin and Silica fume in an optimum proportion proves to be very useful to modify the properties of concrete. This project deals with the properties of concrete, with varying percentage replacement of Silica fume and Metakaolin as a partial replacement for cement. The mix was obtained by replacing (35%, 15%); (40%, 10%) and (45%, 5%) mass of cement by Silica fume and Metakaolin respectively. Finally required specimens were casted to study the behaviors such as compressive strength, tensile strength and durability. Compressive strength and split tensile test were carried out for testing the strength properties and sorptivity test was conducted to check the durability properties of concrete. The test results indicated that the two admixtures Silica fume and Metakaolin when used at an optimum combination tend to increase the strength and durability of concrete when compared with conventional concrete.
Key Words:Silica fume, Metakaolin
Ordinary Portland cement is one of the most important binding materials in terms of quantity produced. Since it is manufactured at a very high temperature, it consumes lot of energy. Besides huge amount of energy consumption, it emits harmful gases, which pollute the atmosphere. The production of every ton of Portland cement contributes about one ton of CO2in the atmosphere. Small amounts of NOxand CH4gases are also emitted. Apart from energy
consumption and emission of harmful gases, calcium hydroxide, one of the hydration products, obtained during the hydration of cement, is a nuisance for construction industry. This affects the durability properties of cement based materials.
Silica fume is an ultrafine powder collected as a by-product of the silicon and ferrosilicon alloy production and natural waste Metakaolinwhich is a dehydroxylated form of the clay mineral kaolinite which when not disposed properly may cause environmental hazards to thesurrounding area. These two materials are usedin the concrete industry, are effective in increasing the compressive strength, tensile strength and improved durability.
II. EXPERIMENTAL INVESTGATION
The cement used for the investigation was Ordinary Portland Cement with 53 grade. The specific gravity of cement is 3.15
Aggregate available from local sources has been used. Aggregate passing through 20mm IS sieve and retained on 16mm IS sieve was used. The specific gravity of coarse aggregate is 2.70.
Locally available river sand of size 2.36 mm was used. The specific gravity of fine aggregate is 2.65, fineness modulus was found to be 2.7 as per IS 383:1970.
Silicafume And Metakaolinarethe mineral admixture used in this work .The physical properties of silicafume are presented in table 1 and The physical and chemical properties of metakaolin are presented in table 2.
TABLE- 1 PHYSICAL PROPERTIES OF SILICAFUME
PROPERTY VALUE SPECIFIC GRAVITY 2.3
PHYSICAL FORM Powder COLOUR Off-White
TABLE-2 PHYSICAL AND CHEMICAL PROPERTIES OF METAKAOLIN
PROPERTY VALUE SPECIFIC GRAVITY 2.6
PHYSICAL FORM Powder COLOUR Off-White INGREDIENTS % BY WEIGHT
Na2O 0.08 Water
Water used for curing and mixingwere as per IS 456:2000.
Fig1Flow chat showing methodology
Fig2 Pie Chart showing Mixing Methodology
Cube and cylinder cast were done. Concrete cubes of size 150 mm x 150 mm x 150 mm and cylinders of size 150mm x 300 mm were cast to study the compressive and tensile strengths. Strength tests of cylinder and cube specimens were performed in Universal testing machineand compression testing machine. Three different mix of specimens were made, in mix 1 cement was replaced by silicafume and metakaolin by 35% and 15% respectively and in mix 2 cement was replaced by silicafume and metakaolin by 40% and 10% respectively and in mix 3 cement was replaced by silicafume and metakaolin by 45% and 5% respectively.
45% 50% 50%
Table -4Mix proportioning
S.NO Parameters Mix Properties
1 Grade of concrete M30 2 Mix Proportion 1:1.01:2.48 3 Cement (kg/m3) 478 kg/m3 4 Fine Aggregate (kg/m3) 519 Kg/m3 5 Coarse Aggregate 1179 Kg/m3 6 Water 191 Kg/m3
III. RESULTS AND DISCUSSION
i)Mean compressive strength
Figure 3 shows the mean compressive strengths of control concrete, (35%, 15%), (40%, 10%) and (45%, 5%) of silicafume and Metakaolin imparted specimens respectively for 7, 14 and 28 days curing. The compressive strength of the control concrete for 7, 14 and 28 days are 24.2 N/mm2, 28.4 N/mm2 and 37.6 N/mm2. For the first mix, that is for the concrete made by replacing cement with 35% silicafume and 15% Metakaolin, the 7 days strength seems to be 29.6 N/mm2, the 14 days strength is 35.4 N/mm2 and the 28 days strength is 43.6 N/mm2. Similarly for the second mix, that is for the concrete made by replacing cement with 40% silicafume and 10% Metakaolin, the strengths are 28.22 N/mm2, 32.8 N/mm2 and 40.24 N/mm2. As for the third mix the strengths are as follows, 25.08 N/mm2, 31.14 N/mm2 and 38.8 N/mm2respectively.
FIG3 BARCHART SHOWING COMPRESSIVE STRENGTH FOR THE THREE MIXES IN N/mm2
ii)Mean tensile strength
40% silicafume and 10% Metakaolin, the strengths are 1.4 N/mm2 and 2.2 N/mm2. As for the third mix the strengths are as follows, 1.2 N/mm2 and 2.0 N/mm2.
FIG 4 GRAPH SHOWING TENSILE STRENGTH FOR THE THREE MIXES
From the obtained values, sorption coefficient is computed values are shown in table 5 and table 6. Low sorption coefficient samples are more impermeable and they show good durability performance Form this short term durability characteristics are found out.
Table-6 Q/A values for the three mixes
The sorption coefficient for control concrete is 3.68x10-2 mm/sec1/2. As for the three mixes the values of sorption coefficients are 1.87x10-2 mm/sec1/2, 2.76x10-2 mm/sec1/2 and 2.84x10-2 mm/sec1/2. It is seen from the results that the sorption coefficient for the three mixes is comparatively less than that of the control concrete. This implies that the durability of the mix-1 that is, for 35% silicafume and 15% Metakaolin is more. The durability of the other two mixes is also high than the control concrete. Of the three mixes the better durability is obtained for the mix I.
It was observed from the test results that the compressive strength and tensile strength of concrete cubes replaced with silicafume and Metakaolin showed better results compared with control concrete. The two admixtures silicafume and Metakaolin when used at an optimum combination of (35%, 15%) respectively, tend to increase the compressive strength of concrete. Thereafter there is slight decline in strength for (40%, 10%) and (45%, 5%) combinations, but not less than that of the target mean strength. It was observed from the test results that the tensile strength of concrete cylinders replaced with silicafume and Metakaolin at an optimum combination of (35%, 15%) showed better results compared with control concrete. Also the two admixtures silicafume and Metakaolin when used at an optimum combination of (35%, 15%) respectively, tend to increase the durability of concrete. The test results indicated that the two mineral admixtures silicafume and Metakaolin when used at an optimum combination of (35%, 15%) respectively tend to increase the strength and durability of concrete when compared with conventional concrete. Therefore the best combination of Metakaolin and silicafume is 35% and 15%.
 An Cheng, Ran Huang, Jiann-Kuo Wu and Cheng HainChenl , “ Influence of GGBS on durability and corrosion behavior of reinforced concrete”, Materials Chemistry and Physics 93, 404–411,2005.
 CananTasdemir, “ Combined effects of mineral admixtures and curing conditions on the sorptivity coefficient of concrete”, Cement and Concrete Research, 33, 1637–1642,2003.
 Deepa Sinha, A, “ Comparative mechanical properties of different ternary blended concrete”, Indian journal of research, volume 1(10),65-68,2007.
 ErhanGu¨neyisi, KasimMermerdas and Mehmet Gesoglu, “ Improving strength, drying shrinkage, and pore structure of concrete using metakaolin”,2007.
 HanifiBinici, OrhanAksogan, Ismail Cagatay, H., Mustafa Tokyay and EnginEmsen, “ The effect of particle size distribution on the properties of blended cements incorporating silicafume and natural pozzolan”, Powder Technology 177 ,140–147,2007.
 IS: 383- IS:
456- IS: 10262- lines for Concrete Mix Design.
 Patil, B.B., and Kumbhar, P.D , “ Strength and Durability Properties of High Performance Concrete incorporating High Reactivity Metakaolin”, Volume 2(3), 1099-1104,2012.